**HAL Id: hal-03169518**

**https://hal.archives-ouvertes.fr/hal-03169518**

Submitted on 15 Mar 2021
**HAL is a multi-disciplinary open access**

archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

**Probabilistic Failure Analysis, Performance Assessment,**

**and Sensitivity Analysis of Corroded Reinforced**

**Concrete Structures**

### Hongyuan Guo, You Dong, Emilio Bastidas-Arteaga, Xiang-Lin Gu

**To cite this version:**

Hongyuan Guo, You Dong, Emilio Bastidas-Arteaga, Xiang-Lin Gu. Probabilistic Failure Analy-sis, Performance Assessment, and Sensitivity Analysis of Corroded Reinforced Concrete Structures. Engineering Failure Analysis, Elsevier, 2021, pp.105328. �10.1016/j.engfailanal.2021.105328�. �hal-03169518�

**Probabilistic Failure Analysis, Performance Assessment, and Sensitivity Analysis of **
**Corroded Reinforced Concrete Structures **

Hongyuan Guo1,2,3_{, You Dong}1,*_{, Emilio Bastidas-Arteaga}4, 5_{, and Xiang-Lin Gu}2,3

1. Department of Civil and Environmental Engineering, The Hong Kong Polytechnic University, Hong Kong, China

2. Key Laboratory of Performance Evolution and Control for Engineering Structures of Ministry of Education, Tongji University, 1239 Siping Rd., Shanghai 200092, China

3. Department of Structural Engineering, College of Civil Engineering, Tongji University, 1239 Siping Rd., Shanghai 200092, China

4. University of Nantes, GeM UMR CNRS 6183, Nantes, France 5. La Rochelle University, LaSIE UMR CNRS 7356, Nantes, France

**Abstract: A better understanding of the mechanical performance and the failure modes of **

corroded reinforced concrete (RC) structures is crucial for implementing measures that reduce failure risks. Therefore, this paper proposes a probabilistic numerical framework to estimate the structural performance and to identify the failure modes as well as the main influencing parameters affecting the safety of corroded RC structures. This framework comprehensively combines experimental data, finite element method (FEM), and polynomial chaos expansion (PCE) modeling. First, the FEM for failure analysis is developed and verified with a 26-year-old corroded RC beam. The investigated case considers the effects of corrosion degree and bond behavior of the steel-concrete interface on the mechanical properties and failure mode of the corroded RC beam. Second, PCE surrogate models for serviceability and ultimate limit states are established by combining the sampling technique (e.g., Sobol sequences) and the validated FEM model. Finally, a global sensitivity analysis is conducted using the PCE model. Several illustrative cases are presented to analyze, in deterministic and probabilistic manners, the failure modes and the sensitivities of material properties and geometry characteristics for both serviceability and ultimate limit states. The results of this study could provide useful insights for understanding the main failure modes of RC structures under different corrosion scenarios.

**Keywords: Reinforced concrete structure; polynomial chaos expansion; global sensitivity **

analysis; failure analysis.

**** _{ Corresponding Author }**

E-mail address: you.dong@polyu.edu.hk

Please cite this paper as:

Guo H, Dong Y, Bastidas-Arteaga E (2021). Probabilistic Failure Analysis, Performance Assessment, and Sensitivity Analysis of Corroded Reinforced Concrete Structures. Engineering Failure Analysis. Article ID: 105328

**List of acronyms **

FEM: Finite element method MCS: Monte Carlo simulation PCE: Polynomial chaos expansion RC: Reinforced concrete

RSM: Response surface method SA: Sensitivity analysis SLS: Serviceability limit state ULS: Ultimate limit state

**1 Introduction **

Under aggressive chloride-contaminated environments, reinforcement corrosion might occur, reducing the serviceability and safety of reinforced concrete (RC) structures and further causing a long-term impact on society and the environment [1–3]. A survey published by NACE International indicated that the global cost of corrosion is around 2.5 trillion US dollars, which corresponds to about 3.4 % of global Gross Domestic Product in 2013 [4]. Thus, concerning the high corrosion cost, it is of great importance to raise awareness of improved maintenance practices that reduce cost, environmental and social impacts. Towards this aim, a robust and unified assessment methodology for the performance assessment of RC structures needs to be proposed.

Failure analysis and performance assessment of corroded RC structures are based on
deterministic and probabilistic approaches. Experiments [5,6], analytical methods [7], and
finite element methods (FEM) [8,9] are typically used in deterministic studies. For instance,
*Ye et al. [6] conducted an experimental failure analysis of 13 corroded RC beams and found *
that these beams could fail by shear when the corrosion level of stirrups reaches a critical
value. Experiments could provide reliable and intuitive findings for model validation and/or
lifetime modeling but are usually time-consuming and costly. Thus, many scholars proposed
analytical models to perform the failure analysis for corroded RC structures. For instance,
*Recupero et al. [7] developed an analytical model to predict the shear and flexural capacity of *
RC elements and validated it with a data set of experimental results. However, due to the
difficulty in depicting the complex mechanisms of reinforcement corrosion and structural

behavior, the analytical models generally deviate significantly from the experimental results.
Owing to the rapid development of computing technology, FEM has also been applied to
simulate and evaluate the structural performance in time with high accuracy [10]. For
*example, Kallias et al. [8] applied FEM for sensitivity analysis (SA) to investigate the effects *
of concrete strength and bond deterioration on the performance of corroded RC beams. Thus,
deterministic analysis has been successfully adopted in the performance evaluation and
failure analysis of corroded RC structures.

Considering the uncertainties and spatial variability inherent to the surrounding
environmental conditions, deterioration processes, models, and material properties, it is a
requirement to conduct a comprehensive failure/performance analysis of corroded RC
structures [11,12]. Therefore, the probabilistic analysis methods applied to corroded RC
structures attracted the attention of scholars and engineers [13]. Many scholars applied
analytical models and/or Monte Carlo simulation (MCS) to carry out probabilistic analyses
[14,15]. For instance, Li and Melchers [16] utilized a probabilistic analytical model to carry
out a SA to determine the critical parameters for the corroded RC beam. Other studies [15,17]
considered pitting corrosion and performed reliability analysis with respect to the spatial
variability of a corroded RC beam. However, the models mentioned above might neglect
some critical information, such as the bond behavior of corroded reinforcement [18],
deflection, cracking patterns on RC beam [19]. Many scholars adopted probabilistic
*FEM-based approaches [18,20] to address the above issues. Bergmeister et al. [21] proposed *
a probabilistic assessment framework based on Latin hypercube sampling and non-linear
*FEM to perform sensitivity and reliability analysis. Zhang et al. [18] carried out a reliability *
estimation of a corroded RC beam by using FEM and X-ray photographs to account for the
spatial variability of corroded steel bars.

The FEM-based probabilistic analysis could provide reliable and comprehensive lifetime assessments; however, a realistic prediction might also impose a significant computational burden due to the complexity of the numerical models, including a set of non-linear and coupled differential equations, resolutions in space and time, and a large number of

parameters. Thus, surrogate models are useful tools for alleviating computational costs in
FEM-based probabilistic analysis. Among these models, statistical methods, such as the
response surface method (RSM), were intended to establish a surrogate model for a RC beam
to reduce the cost of MCS [18] and conduct SA [22]. However, studies have shown that RSM
may not be feasible for analyzing global sensitivity due to its limited accuracy [23].
Polynomial chaos expansion (PCE) based probabilistic analysis methods have received
extensive attention due to their high accuracy and efficiency in establishing surrogate models
[24,25]. In addition, PCE-based methods allow the SA of random variables, i.e., global SA,
by integrating full randomness and variability of input and output variables. However, few
studies have been done in PCE-based probabilistic analysis for corroded RC structures. For
*instance, Bastidas-Arteaga et al. [25] developed a PCE-based probabilistic model for global *
SA of RC structures suffering from chloride-induced corrosion, but their study focused on the
initiation period (Serviceability limit state, SLS) rather than the propagation period (Ultimate
limit state, ULS). Thus, it is of vital importance to conduct a complete analysis of structural
performance, considering both SLS and ULS.

In this study, we propose a comprehensive framework for probabilistic failure analysis, performance assessment, and sensitivity analysis of corroded RC structures. It combines experimental data, FEM, and PCE. We particularly focus on existing corroded RC structures where the current corrosion condition of rebars and the presence of cracks provide more uncertainties to the performance assessment at the moment of the inspection and/or the evaluation of the remaining capacity. The basic concepts and algorithms of the proposed framework are introduced in Section 2. Then, in Section 3, using a corroded RC beam as one example, the FEM model is established in detail. The principles and algorithms of PCE are introduced in Section 4. Section 5 presents the results associated with the illustrative example. The first subsection in Section 5 verifies the feasibility and accuracy of the proposed FEM model based on a study of a 26-year-old corroded RC beam. The second subsection focuses on the development of the PCE and its application for sensitivity and failure analyses.

**2 Performance assessment and failure analysis of corroded RC structures **

In this study, the performance assessment of corroded reinforced concrete (RC) structures focuses on different components of the structural response, such as the curves of external loads versus deformations, the distribution of reinforcement stresses, and concrete strains, and cracking patterns. Based on the structural response, the evolution of the RC structures under external loads can be studied; the limit states of RC structures, including the serviceability limit state (SLS) and ultimate limit state (ULS), can be determined; and more importantly, the potential failure mode and pattern could be deduced.

**The general computational framework of performance assessment is presented in Fig. 1. **
As indicated, the proposed framework consists of ten steps. The first two steps are the
determination of geometric and mechanical information of the RC structure (e.g., remaining
cross-sectional section of rebars and the presence of cracks, among others.), which depends
on the investigated example. In this paper, the information is obtained from experiments to
validate the numerical results. Due to the experimental costs, it is not feasible to conduct a
large number of experiments, so that numerical analysis is needed to perform failure analysis
by considering different scenarios. The main inputs of this numerical analysis are the
geometry information, constitutive models of concrete, corroded steel bars, and bond-slip,
boundary conditions, among others. The third step is to perform finite element method (FEM)
simulation using commercial FEM software, DIANA 10.3 [26], to account for the
above-mentioned parameters. Other software could also be adopted within the structural
analysis process. Detailed processes associated with FEM, including geometry modeling and
material constitutive models, are introduced in Section 3.

**Fig. 1. General framework for performance assessment of corroded RC structures **

The third to sixth steps are devoted to perform deterministic analysis, and the primary goal is to demonstrate the applicability and accuracy of numerical models by comparing them with experimental data, i.e., the fourth step. The information on the geometry and mechanical parameters of the corroded RC beam is mainly derived from the first and second steps, i.e., experimental studies on existing structures. Apart from the experimental verification in the fourth step, different assumptions (e.g., corrosion degree of reinforcement and constitutive models of materials) are made and assessed. The fifth step (failure analysis) is conducted to investigate the failure mechanisms. Subsequently, the sixth step, i.e., local sensitivity analysis (SA), is performed to study different parameters on structural performance (e.g., the effect of corrosion degree on structural behavior and the spatial effect on stress and crack distribution).

On the other hand, probabilistic analysis (the seventh to tenth steps) is needed to account for the uncertainties associated with different variables. For instance, in the seventh step, some geometrical parameters (e.g., the geometry of corroded rebar) are represented by probabilistic models (Section 3.1.2). In this study, a low discrepancy sequence-based Monte

**Experiment**
① Geometric information
② Mechanical information
**Deterministic analysis**
③ FEM modeling
④ Computation verification
**Probabilistic analysis**

⑤ Deterministic failure analysis

⑦ Probabilistic modeling ⑧ Surrogate modeling

⑩ Global sensitivity analysis ⑥ Local sensitivity analysis

Carlo simulation (MCS) (e.g., Sobol sequences) is conducted to generate critical information of the FEM model and perform the FEM analysis. However, brute MCS is computationally expensive, and global SA is not easy to be conducted. To tackle this problem, a surrogate model (Section 4) is established in the eighth step. In this study, polynomial chaos expansion (PCE) is employed for the surrogate modeling due to its high accuracy and efficiency in global SA as the sensitivity factors could be computed directly through the coefficients of PCE. Then, the built surrogate model is employed in the ninth and tenth steps for probabilistic failure analyses and global SA, respectively.

**3 FEM model of a corroded RC beam **
**3.1 Spatial variability of corroded rebars **

In this study, a corroded reinforced concrete (RC) beam is used as an example to illustrate the
**proposed methodology. As shown in Fig. 2, the length and cover thickness of the beam are L ***and c, respectively, and the cross-sectional width and height are denoted as b and h, *
*respectively. The reinforcement layout of this RC beam is: nt tension bars, n*c compression
*bars, and n+1 stirrup bars with n*sv* vertical legs and sv* stirrup spacing. Deterministic and

probabilistic approaches could be implemented to consider the spatial variability of corroded rebars. Both approaches are summarized in the following sections.

**Fig. 2. Geometry schematic of the RC beam **
*3.1.1 * *Deterministic modeling *

Deterministic modeling is commonly used in experimental validations [9,27]. In previous studies, the geometry of corroded steel bars is represented by a cylinder with a reduced diameter. Also, based on the assumption of uniform corrosion, the corrosion degree is

*L *
*sv*
*b *
*h *
*nt*tension bars
*n*ccompression bars
*nsv*vertical legs
*c*

*quantified by an average corrosion degree η*ave [28]. However, non-uniform and pitting
corrosion are common phenomena in practice, which would induce spatial variability and the
*local corrosion degree η*s [15]. Thus, it is necessary to establish a spatial variability model of
non-uniform corrosion accounting for the previously mentioned effects.

Characterizing the spatial variability of corroded rebars is not an easy task. To date, at least three methods, based on experimental procedures, have been used to achieve this goal, as follows:

(1) to cut the entire corroded steel bar into several segments along its axis, then to measure the mass of each segment and finally obtain the distribution of mass loss ratio along the axis [29];

(2) to measure the residual diameter of steel bar along the axis using a Vernier caliper, then to compute the distribution of diameter loss along the axis [30]; and

(3) to employ a three-dimensional light scanner [31] or X-ray photograph [18] to obtain a 2D/3D geometry model of corroded steel bars directly and then analyze the distribution of cross-sectional areas.

The first method could reflect the gravimetric loss of steel bars but damages the specimen. The third method could reveal the complete geometry information of the steel bar with relatively high accuracy; however, the used measurement devices are relatively expensive, and advanced numerical methods are required to analyze the output. In order to balance measurement accuracy and experimental cost, the second method is usually regarded as a compromise choice, which is convenient to be used in practical engineering. Also, the Vernier caliper is a cheaper tool than the devices in the third method, and it causes less damage to the structure compared with the first method.

Once the spatial geometry of the corroded steel bar is obtained, the spatial variability of
longitudinal (tension and compression) bars would be simplified to a series of bar elements
with different circular cross-sections as the input for the finite element method (FEM) model.
*For the n*t* tension bars and n*c compression bars, the first step is to divide each longitudinal
*bar into n zones. Then, at the i-zone, the maximum diameter loss of j-th tension bar, pt, max,i,j*

*and k-th compressive bar, pc, max,i,k* are measured and then used to calculate the minimum
cross-sectional areas by Eqs. (1) and (2). Thus, the cross-sectional areas of the bar elements
*within each zone and longitudinal bar, i.e., cross-sectional area of tension bars, At,i,j (i = 1, *

*2,…, n and j = 1, 2, ..., nt) and compression bars, Ac,i,k (i = 1, 2,…, n and k = 1, 2, …, n*c), are
*represented by their minimum cross-sectional area. For the n+1 stirrup bars, each stirrup bar *
*is divided into n*sv* vertical legs. Next, at the l-th vertical leg, the maximum diameter loss *

*psv,max,m,l at the m-th stirrup bar is also measured to compute the minimum cross-sectional area *

*Asv,m,l (m = 1, 2, …, n+1, l = 1, 2, …, n*sv) by Eq.(3).

(1)
(2)
(3)
*in which Dt0, D*c0*, and D*sv0 are the expected diameters of uncorroded tension bar,
*compression bar, and stirrup, respectively. Also, local corrosion degree η*s could be quantified
by the difference ratio between the original and the minimum cross-sectional area from
Eqs.(1)-(3).

Besides, to evaluate the bond strength between the steel-concrete interface, the surface
*area of steel bar A*surf of the corroded steel bar can be computed as

(4)

*where p, D*0*, and L*bar, denote the diameter loss due to corrosion, initial diameter, and
longitudinal length, respectively.

*3.1.2 * *Probabilistic modeling *

A probabilistic approach is more suitable to account for the spatial variability of corroded rebars geometry in a more realistic way. The corroded geometry could be defined by the pitting factor, which is the ratio of the maximum pit depth to the average pit depth of the corroded steel bar [32]. By employing the Type-I extreme distribution, Stewart and Alharthy [15] developed the probabilistic model of pitting factor to conduct reliability analysis. Besides, Darmawan [33] improved the model of pitting factor by considering time parameters

## (

## )

2 , , 0 ,max, , 4*t i j*

*t*

*t*

*i j*

*A*=p

*D*-

*p*

### (

### )

2 , , 0 ,max, , 4*c i k*

*c*

*c*

*i k*

*A*=p

*D*-

*p*

### (

### )

2 , , 0 ,max, , 4*sv m l*

*sv*

*sv*

*m l*

*A*=p

*D*-

*p*

### (

0### )

*surf*

*bar*

*A*

### =

### p

*D*

### -

*p L*

and corrosion rates. However, the pitting factor-based probabilistic model assumes one-single
pit. Later, some scholars have made some improvements in the stochastic modeling of the
*corroded steel bar. For instance, Tang et al. [34] proposed to use a mixed normal distribution *
to model the cross-sectional area, but it neglects longitudinal correlations.

On the other hand, considering the complex geometry and random distribution of pits in
*the cross-section of a corroded steel bar, Gu et al. [12] proposed the corrosion non-uniformity *
*factor, R, defined as the ratio of the average cross-sectional area to the minimum *
cross-sectional area, i.e.,

(5)
*in which Aav and A*min are the average cross-sectional area and the minimum cross-sectional
*area, respectively; η*ave* is the average corrosion ratio of the steel bar; and D*0 is the initial
*diameter of the rebar. Factor R also follows the Type-I extreme distribution, and distribution *
*parameters μ and σ could be computed by [11,12] *

(6)
(7)
*where i*corr* (μA/cm*2*) is the corrosion current density; and As* (mm2*) and As0* (mm2) are the

surface areas of the Lbar* and 50 mm length of steel bar. *

(8)
*For tension and compression bars, L*bar can be determined by the length of each zone,
*while for stirrup bars, the L*bar can be determined by the vertical height of the stirrup leg. The
*factor R and the minimum cross-sectional area of each element are statistically independent *
*of the others. Given the samples of factor R and other parameters, e.g., i*corr* and n*ave, the
minimum cross-sectional areas of corroded steel bars could be computed through Eq. (5), and
assigned into different elements of steel bars.

2
min 0(1 ) min
*av* *ave*
*R A*= *A* =p*D* -h *A*

### (

### )

s s 0 3.35 exp 0.236*i*0.12 ln( /

_{corr}*A A*

_{s}*) 1.01*

_{s}### µ

=### h

- +### h s

+ +### 0.3371

_{s}### 0.0006

### s

### =

### h

### +

0### ,

0### 50

0*s*

*bar*

*s*

*A*

### =

*L*

### p

*D A*

### =

### p

*D*

**3.2 Constitutive model of materials **
*3.2.1 * *Concrete *

The total strain-based crack model is applied for the constitutive model of concrete, which is based on total strain and the modified compression field theory [35]. In this model, the stress-strain relationship is evaluated in the principal directions of the strain vector, i.e., the coaxial stress-strain concept. In terms of the relationship between the directions of crack and principal stress, two types of crack models are presented:

(1) Fixed crack model, in which the crack direction would not change with the principal stress once cracking happens.

(2) Rotating crack model, in which the crack direction would keep changing with the principal stress.

In the fixed crack model, the shear resistance of the cracks is modeled by the shear retention factor, reflecting the aggregate interlock effect caused by cracked concrete. In the rotating crack model, there exist no shear stresses on the crack plane, which simplifies the analysis and receives a large scale of application [36,37]. This study applies the rotating crack model.

**Tensile and compressive behaviors of concrete are illustrated in Fig. 3. For the tensile **
behavior of concrete, the stress increases linearly before reaching the ultimate tensile strength.
Then, it drops following a tension softening model developed by Hordijk [38]. For the
compressive behavior of concrete, the stress increases/decreases following parabolic curves
**[39], as shown in Fig. 3. **
**Notation: **
*f _{t}*

*f*

_{c}*ε*

_{tu}*G*

_{ft}/h_{el}*G*

_{fc}/h_{el}*ε*

_{cu}*Gft*: tensile fracture energy;

*Gfc*: compressive fracture energy;

*ft*: ultimate tensile stress;

*f*c: ultimate compression stress;

𝜀*tu*: ultimate tensile strain;

𝜀*cu*: ultimate compression strain;

*hel*: ‘equivalent length’ relating to

element type and element size, among
**others. [39] **

**Fig. 3. Schematic of the constitutive model of concrete **

The ultimate tensile and compression strains are computed by the tensile and
*compressive fracture energies Gft and Gfc (kN/m), respectively. Gft* can be calculated by a

formula proposed by FIB Model Code 2010 [40]

(9)
*In this study, the compressive fracture energy Gfc* is supposed to be about 100 times of

*Gft* [39]. A reduction factor is proposed to consider the influence of cracking on the

compressive strength [41], and the lower bound of the reduction factor is assumed as 0.6 in this study.

*3.2.2 * *Corroded reinforcement *

In general, the corrosion of a RC beam affects not only the geometry but also the constitutive
model of the steel bars. In most of the available studies, the constitutive models of steel bars
supposed that yield and ultimate strengths would reduce with corrosion degree [2,8].
However, previous studies proved that corroded reinforcement might fail at the location of
the minimum cross-sectional area, and its actual strength does not change if the stress at the
broken section is taken to measure its strength [12]. Besides, in previous studies related to the
FEM analysis of corroded RC structures, reinforcement is usually modeled by bilinear/ideal
elastoplastic constitutive models to simplify the stress-strain relationship [8,42]. However,
the deformation ability and nominal strength of corroded reinforcement (nominal strength is
the yield/ultimate tensile force divided by the uncorroded cross-sectional area or average
cross-sectional area) decreases significantly with corrosion degree [43,44]. Studies showed
that the failure mode of corroded steel bar would change from ductile failure to brittle failure
*once its corrosion degree η*s exceeds about 20 ~ 30% [45,46].

In this study, by combining the existing studies in [12,45], a new trilinear constitutive
**model of corroded steel bars is proposed, as depicted in Fig. 4. Given that the elastic modulus **

0.18

0.073

*ft* *c*

*E*s0*, actual yield strength f*y0*, and ultimate strength of corroded steel bar fu0* remain unchanged,

the harden strain and ultimate strain decrease with the corrosion degree. The evolution of the constitutive relationship of a corroded steel bar subjected to tension is described by Eqs. (10) and (11) [47]. For reinforcement, the Von Mises plasticity model is used, assuming isotropic hardening.

(10)

(11)
*where η*s,cr* is the critical corrosion degree (20 ~ 30% [45]); εsh0 and εsu0* are the harden strain

and ultimate strain of non-corroded steel bar; ε*shc and εsuc* are the harden strain and ultimate

strain of corroded steel bar; and βδ = 2.093 and 2.501 for salt spray induced corrosion and natural corrosion (corroded steel bars obtained under real environmental conditions), respectively [48].

**Fig. 4. Constitutive models of corroded steel bars. **
*3.2.3 * *Bond-slip *

If a RC beam is well-anchored and no corrosion happens, the reinforcement could be supposed to be well embedded inside the concrete. Otherwise, bond-slip behavior must be considered in the FEM. The bond-slip relationship could be assigned to the interface between

0 0
0 ,
0 0 ,
,
0
1 ,
,
*y* *y* *s*
*sh* *s* *s cr*
*s* *s* *s cr*
*shc*
*yc*
*syc* *s* *s cr*
*s*
*f* *f*
*E* *E*
*f*
*E*
h
e h h
h
e
e h h
ì æ öæ ö
+ - - £
ï ç _{÷ç}ç ÷_{÷}
ï è øè ø
= í
ï _{=} _{>}
ï
î

### (

### )

0 exp ,*suc*d

*s*

*su*

### e

= -### b h e

*η*s

*σsc*

*εsc*

*εsu0*

*εsh0*

*εsy0*

*εsuc*

*εshc*

*εsyc*

*fu0*

*fy0*

the steel bar and concrete directly. Employing the bond-slip model proposed by Kallas and
*Rafiq [8], the bond stress τ versus slip s could be described as follows *

(12)

*where α and β denote the factors of the bond model (i.e., α = 0.7 and β = 0.3); l*0*, l*1*, and s*2 are
*0.4 mm, 0.15c*0*, and 0.35c*0* (c*0 is the rib spacing, e.g., 8 mm [8]), respectively; and 𝜏max is the
maximum bond strength of concrete beam with deformed rebars. In this study, 𝜏max is
evaluated by an empirical model [49]:

(13)

*where c is the cover thickness of concrete; d*b is the diameter of the deformed tension rebar;

*Asv is the cross-sectional area of stirrup bars; sv is the stirrup spacing; and k*1* and k*2 are the
empirical factors accounting for the reduced contribution of concrete towards bond strength,
relating to the corrosion current density of steel bar. For the corrosion current density of 40
µA/cm2_{, k}

1 *and k*2 are 1.003 and -0.037 [50], respectively; For the corrosion current density of
90 µA/cm2_{, k}_{1 }_{and k}_{2}_{ are 1.104 and -0.024 [50], respectively. }

**4 Surrogate model and global sensitivity analysis **
**4.1 General description **

To conduct the global sensitivity analysis (SA), the finite element method (FEM) is combined with polynomial chaos expansion (PCE) surrogate modeling using the MATLAB® software.

**Fig. 5 describes the methodology used to create the surrogate models. Monte Carlo **

*simulation (MCS) is used to propagate uncertainty in FEM and generate N input and output *
variables necessary to build the PCE surrogate model presented in Section 4.2. In this process,
it is necessary to determine the distributions of random input variables (e.g., material
mechanical parameters, the cross-sectional area of steel bar), output variables (e.g., ultimate

### (

### )

### (

### ) (

### ) (

### )

### (

### ) (

### ) (

### )

### (

### )

### [

### ]

### (

### )

0.3 1 1 0 0 1 0 max max 0 1 1 1 2 max max 1 2 1/0.3 0.5 1 0 1 max 1 1 1 max 1 0 1 max / ,0 1 , , 1 , 2.57 , , exp (1/ 0.3) ln( / ) ln /*c*

*s l*

*s s*

*s s*

*s*

*s*

*s*

*s s*

*s s*

*s*

*s*

*s*

*s s*

*f*

*s*

*l*

*s*

*l*

*l*t t a t a t b t t t at t t t t t ì

_{£ <}ïï =

_{í}- - × - × + × £ < ï - - × - × + £ < ïî = = = +

### (

### )

### (

### )

### (

### )

max*k k*

1 2 *s*

### 0.55 0.24 /

*c d*

*b*

*f*

*c*

### 0.191

*A f*

*sv y*

*s d*

*v*

*b*

### t

### =

### +

### h

### é

_{ë}

### +

### ù

_{û}

### +

### ×

### ×

and serviceability capacity indicators). Meanwhile, a type of low discrepancy sequence, Sobol nets [51], is employed to improve the sampling efficiency. Once the PCE model is established, SA could be carried out through the approaches described in Sections 4.3, respectively.

**Fig. 5. Establishment processes of PCE **

**4.2 Surrogate modeling: polynomial chaos expansion **

The idea of PCE is to establish a surrogate model Γ*PCE* by expanding the target response onto

**the basis of the probability space from input variables. All uncertain input variables x = ***{x*1*,…, xN*} should be represented by a marginal probability density function (PDF) [52].

* Meanwhile, the system response g(x) could be approximately replaced by an orthogonal *
polynomial basis Γ

*PCE*

_{ [53] }

(14)

*where Ii*1*,…,i*M* denotes the set of non-zero indices (i*1*,…, i*M*); aj and p are the coefficient and *

order of PCE, respectively; and Ψ*j (x) is the product of one-dimensional polynomials ϕaj*.

Determine input and output random
*variables and the sampling number N*

*i = 1*

Sample a series of input variables then
*conduct the i-th FEM simulation*
*Extract the output variables from i-th*

FEM simulation
*If i = N?*

*i = i+1*

Reorganize all input and output variables then Establish PCE

* Sobol net-based MCS*
Yes
No

### ( )

_{1}

_{2}1 2 1 2, 1 1 1 1,..., 1,..., 1 0 0 1 1 1 ... ( ) ( ) ( , ) ... ( )! ( ,..., ) ... ( ,..., ), ! !

*i*

*i i*

*s*

*M*

*s*

*i*

*is*

*i*

*iM*

*M*

*M*

*PCE*

*j*

*j*

*j*

*j*

*j*

*j*

*j*

*i*

*i*

*j*

*i*

*j I*

*i i M j I*

*j*

*j*

*i*

*i*

*j*

*j*

*i*

*i*

*i*

*i M j I*

*j I*

*g*

*a*

*a*

*a*

*x*

*a*

*x x*

*N p*

*a*

*x*

*x*

*a*

*x*

*x*

*M*

*N p*-= = Î £ £ £ Î £ £ £ £ Î Î » G = Y = + Y + Y + + + Y + + Y =

## å

## åå

## å å

## å å

## å

**x**

**x*** Supposing the random variables within x follow independent standard normal distributions, *
Ψ

*j*

**(x) in Eq. (14) could be written as a multi-dimensional Hermite polynomial:**(15)
*where ϕaj(xj*) is the one-dimensional Hermite polynomial. The unknown coefficients in Eqs.

(14) and (15) could be determined by the regression approaches [23], e.g., Ordinary Least
Squares (OLS) and Orthogonal Matching Pursuit (OMP) [54], among others. The PCE is
founded on the regression approaches and a training set generated by MCS. More detailed
information on the algorithm is available in [54]. The accuracy of the established PCE could
*be quantified by R*2 * _{or leave-one-out coefficient. Herein, a test set is used to evaluate the R}*2

_{ of }the proposed PCE:

(16)

*where Ntest is the size of the test set, and Γ denotes the system response of MCS. Once the R*2

of PCE satisfies a given requirement, the PCE could be further used in SA.

**4.3 PCE-based global sensitivity analysis **

*In this study, SA is conducted by estimating the Sobol’ indices Si*1*,…,is*, which could determine
the contribution of random input variables (e.g., geometry and mechanical factors) to the
variability of the system response [55]

(17)

*where D and Di*1*,…,is are the total and partial variances of g(x), which can be computed by Eq. *

(18) and (19), respectively. (18) (19)

### ( )

## ( )

1 0*j*

*N*

*j*

*j*

*j*

*j*

*x*a f a = Y

*=*

**x**### Õ

， ³## ( )

## ( )

### ( )

### ( )

## ( )

## ( )

2 2 1 2 1 1 1/ 1 , 1 1*test*

*test*

*test*

*N*

*i*

*PCE*

*i*

*test*

*i*

*N*

*N*

*i*

*i*

*i*

*i*

*test*

*test*

*N*

*R*

*Var*

*Var*

*N*

*N*= = = éG - G ù ë û = -G é ù G =

_{ê}G - G

_{ú}ë û

### å

### å

### å

**x**

**x**

**x***1,...,*

**x***s*1,...,

*s*

*i*

*i*

*i*

*i*

*S*=

*D*

*D*2 2 0 1,2,..., 1 1 Var[ ( )]

*N*( )

*N*

*i*

*ij*

*N*

*K*

*i*

*i j N*

*D*

*g*

*g*

*d*

*g*

*D*

*D*

*D*= £ < £ =

*=*

**x**_{ò}

*- =*

**x x**### å

+### å

+ +!## (

## )

1 1 1 1 2 ,...,*s*

*s*,...,

*s*,....,

*s*....

*s*,1 1 ... , 1,...,

*i*

*i*

_{K}*i*

*i*

*i*

*i*

*i*

*i*

*s*

*D*=

### ò

*g*

*x*

*x dx*

*dx*£ < < £

*i*

*i*

*N s*=

*N*

*where g*0* is the expected value of g(x) and the integral of each summand gi1*...,

*is*is equal to 0.

(20)

where the notation ∼ means the excluded variables and x~i denotes

(21)

According to Eq.(18), there exists

(22)

*where S*i are the first-order indices only containing the influence of every single parameter.
*To consider the interaction effects of different parameters, total sensitivity indices STi* could

be computed as [56]

(23)

*in which S~i is the sum of Si1,…,is without i. In general, it is challenging to calculate Sobol’ *

indices analytically, especially when using complex non-linear deterioration models such as
the described in section 3. Then, MCS could usually be applied to compute Sobol’ indices
with a high computational cost. However, once PCE is set up, Sobol’ indices could be easily
obtained by the coefficients of PCE directly[53]. Based on the definition of Sobol index (Eq.
*(17)), Si*1,…,*i*s could be rewritten as [23]

(24)
*where E(∙) denotes the expectation of (∙). Moreover, Si and STi* could be calculated by

(25)

*where I**

*i denotes the set of all indices in the i-th element. *

### ( )

### ( )

### ( )

## (

## )

### ( )

1 1 0_{0}

_{0}~ 0 1 1 ~( ) 0 0 0 , ... , , ... ( ) ( )

*i*

*i*

*i*

*ij*

*i*

*j*

*ij*

*i*

*i*

*j*

*j*

*g*

*g*

*d g x*

*g*

*d*

*g*

*g x x*

*g*

*d*

*g*

*g x*

*g x*= = -= - -

### -ò

### ò ò

### ò ò

**x x**

**x x**

**x x**### (

### )

~*i*=

*x*1,....,

*xi*-1,

*xi*+1,...,

*xM*

**x**1,2,..., 1 1 1

*N*

*i*

*ij*

*N*

*i*

*i j N*

*S*

*S*

*S*= £ < £ + + + =

### å

### å

! ~ 1*i*

*T*

*i*

*S*= -

*S*

## ( )

1 ,..., 1 1 1 2 2 ,..., 1 2 2_{( ,..}

_{)}, .,

_{M}*i*

*i*

*s*

*M*

*M*

*i*

*i*

*PC*

*j*

*j*

*j*

*P*

*j*

*j*

*i*

*i*

*j I*

*C*

*S*

*D*

*a E*

*D*

*a E*

*x*

*x*-= Î éY ù ë û = = Y

## å

## å

## ( )

## ( )

1 1_{*}1 2 2 2 2 1 2 2 2 2 1 1 ( ,..., ) ( ,..., ) ,

*i*

*i*

*M*

*M*

*i*

*j*

*j*

*i*

*i*

*j*

*j*

*i*

*i*

*j I*

*I*

*i*

*M*

*T*

*M*

*j*

*j*

*j*

*j*

*j*

*j*

*j*

*S*

*S*

*a*

*a E*

*x*

*a E*

*x*

*E*

*x*

*E*

*a*

*x*Î - -= = Î é ù éY ù

_{ë}Y

_{û}ë û = = Y Y

### å

### å

### å

### å

**5 Illustrative examples **
**5.1 Study case description **

In this study, the developed finite element method (FEM) model is verified using the
experimental data associated with 26-year old corroded and uncorroded reinforced concrete
(RC) beams [30]. Accordingly, the corroded RC beam was subjected to a salt spray
environment (35 g/l NaCl solution) and extern loading for six years. The uncorroded RC
beam was under an environment with 50 % relative humidity and 20°C temperature [30]. The
beams were tested through three-point tests. More detailed information regarding the
**experimental studies can be found in [30]. Fig. 6a shows the schematic of the RC beam with **
a dimension of 3000 mm × 150 mm × 280 mm and a cover thickness of 10 mm. The
reinforcement layout is 2ϕ12 longitudinal bars, 2ϕ6 hanger bars, and 14 ϕ6@220 stirrups.
**The beam is subjected to a concentrated load at its mid-span. Fig. 6b shows the FEM model **
of the RC beam with a mesh size of 15 mm. In the 2D model of the beam, the concrete and
reinforcement are discretized by 2D plane stress CQ16M and truss elements, respectively
**[26]. The geometry and materials parameters are summarized in Table 1 and Table 2, **
respectively. Other parameters related to the load step and equilibrium iteration procedure are
**listed in Table 3, where the load increments are 100 steps for the corroded case and 200 steps **
for the uncorroded case.

(a)
(b)
3000
220
150
14 ϕ6@220
2ϕ12
2ϕ6
10
280
220 220 220 220 220 220 220 220 220 220 220 220
*i = 1 i = 2 i = 3*
*…*
*i = 13*
*i = 12*
*i = 11*
*m = 1 m = 2 m = 3* *m = 12 m = 13 m = 14*
*…*
Zone number
Stirrup number
3000 mm
220
280
70
*P*
100

**Fig. 6. (a) Schematic of RC beam in [30] and (b) layout of FEM model of RC beam in **

DIANA (mesh size = 15 mm)

To account for spatial variability of corroded rebars, the beam is divided into 13 zones
**through the spacing of stirrups (220 mm), as shown in Fig. 6. Reinforcement corrosion is **
quantified by diameter loss [30], and all values of diameter loss are supposed to be zero for
**the uncorroded RC beam. Fig. 7 summarizes the distribution and maximum values of **
diameter loss of longitudinal bars at both sides of the beam and maximum diameter losses of
stirrups at the left and right legs.

**Comparing Fig. 7a with Fig. 7b, it seems that compression bars suffer more severe **
*corrosion than tension bars. Zhu et al. [30] attributed this phenomenon to the poor quality of *
the interface between the compression bars and the concrete, which is related to the “top-bar”
effect. The cross-sectional area of each zone is denoted as the sum of all minimum
*cross-sectional areas, e.g., At, i, Ac, i, and Asv, m*

(26)
*where At,i,j, Ac,i,k and Asv,m,l refer to Eq. (1). For the uncorroded scenario, At, i, Ac, i, and Asv, m*
are 226.20 mm2_{, 56.55 mm}2_{, and 56.55 mm}2_{, respectively, while for the corroded scenario, }
**the relevant values are listed in Table 4. **

**Table 1 Parameters of model geometry **

**Geometry ** **Length (mm) Width (mm) Height (mm) Cover thickness (mm) **

Beam 3000 150 280 10

Load plate 100 150 35 -

Support plate 70 150 35 -

**Table 2 Parameters of material properties in [30] **

**Concrete ** **Reinforcement **

*E*c (MPa) 25600 *E*s (MPa) 273000

Poisson ratio 0.2 Poisson ratio 0.3
*Tensile strength f*t (MPa) 1.88 *Yield strength f*y (MPa) 600

*Compressive strength f*c (MPa) 56 *Ultimate strength f*u (MPa) 800

, , , , , , , , ,
1 1 1
, ,
*t* *c* *sv*
*n* *n* *n*
*t i* *t i j* *c i* *c i k* *sv m* *sv m l*
*j* *k* *l*
*A* *A* *A* *A* *A* *A*
= = =
=

### å

=### å

=### å

**Table 3 Parameters of load step and equilibrium iteration procedure **

**Items ** **Option ** **Value **

**Load **

**Preset point load ** Y direction -0.1 mm

**Scale factor ** - 5

**increments ** - 100 (200)

**Step control ** Arc length Default

**Iterative method **

**Maximum number ** - 200

**Method ** Newton-Raphson Default

**Speed up method ** Line search Default

**Convergence norm **

**Tolerance ** Energy 0.001

**Tolerance ** Force 0.01

**Abort criterion ** Energy

10000

**Abort criterion ** Force

**Fig. 7. (a) Comparison between the distribution of actual and maximum diameter loss for (a) **

tensile bars; (b) compressive bars; and (c) maximum diameter loss of stirrup bars

*Note: pt,max,F and pt,max,B* are the maximum diameter loss of tension bars in the front and back sides;

*pc,max,F and pc,max,B* are the maximum diameter loss of compression bars in the front and back sides;

Table 4 Cross-sectional area of each zone of corroded steel bar (mm2_{) }
**A****sv,1** **A****sv,2** **A****sv,3** **A****sv,4** **A****sv,5** **A****sv,6** **A****sv,7** **A****sv,8** **A****sv,9** **A****sv,10** **A****sv,11** **A****sv,12** **A****sv,13**** A****sv,14**
8.53 28.35 25.76 11.61 28.27 16.63 13.43 12.77 42.43 15.37 22.97 28.92 23.43 8.84
**A****c,1** **A****c,2** **A****c,3** **A****c,4** **A****c,5** **A****c,6** **A****c,7** **A****c,8** **A****c,9** **A****c,10** **A****c,11** **A****c,12** **A****c,13**
35.23 12.76 23.45 20.93 40.15 18.64 12.23 4.3 6.84 19.86 21.79 18.93 2.32
**A****t,1** **A****t,2** **A****t,3** **A****t,4** **A****t,5** **A****t,6** **A****t,7** **A****t,8** **A****t,9** **A****t,10** **A****t,11** **A****t,12** **A****t,13**
143.76 128.4 168.01 194.2 158.57 137.09 165.42 171.95 159.31 166.95 155.37 154.62 157.69

Regarding the bond behaviors between steel bars and concrete, two scenarios are considered: ‘perfect bond’ and ‘poor bond’. The former assumes no slip at the interface between reinforcement and concrete, and the latter considers the constitutive model of bond-slip given in Section 3.2.3.

**5.2 Comparison with experimental data **
*5.2.1 * *Comparisons of P-δ curves *

*The calculation results of load P versus the mid-span deflection δ are obtained and compared *
**with experimental results, as indicated in Fig. 8. In general, it is observed that the P-δ curves ***of FEM are consistent with the experimental ones. The P-δ curves are similar at the initial *
stage but gradually become different with different corrosion conditions and bond
*assumptions. Besides, the upward slope of the P-δ curves for the FEM of the corroded *
scenario is close to that of the uncorroded scenario in the initial stage before concrete
cracking in the tensile zone. The reason is that the corrosion-induced damage on concrete is
*not considered, but it does not influence the subsequent development of the P-δ curve after *
concrete cracking. Also, the bond condition could affect the stress and strain distribution of
concrete and reinforcement and further affect the deflection at the beam mid-span.

*Furthermore, the effect of the constitutive model of reinforcement on the P-δ curve is *
illustrated by employing the traditional bilinear constitutive model (only elastic and
hardening phases) with or without corrosion-induced strain descent. The initial phase of the
*P-δ curve from the bilinear constitutive model agrees well with the other curves, but the *

*critical loads such as P*y* and P*u are higher, and the ultimate deformation is lower than other
*scenarios. Besides, P*u of the scenario without the strain descent is higher than other cases,
and its ultimate deformation is slightly higher than the experimental result and the ‘poor bond’
scenario. For the uncorroded RC beam, the effect of the constitutive model of reinforcement
*on the P-δ curve appears to be insignificant, whereas it is larger for the corroded RC beam. *
Therefore, the bilinear constitutive model of reinforcement seems inappropriate, while the
*proposed constitutive model yields a P-δ curve that is closer to the experimental results. *

**Fig. 8 P-δ curves of FEM and experimental data **

*(Dotted black line denotes the serviceability limit deflection L*s = beam length / 500)

*In the following analysis, P*s* is the load for the serviceability limit deflection (L*s = beam
*length/500); the yield load Py and deflection δy indicate the inflection point of the P-δ curve; *

*and the ultimate load Pu and deflection δu are related to the peak point of the P-δ curve. It is *

* noted in Fig. 9 that Py, δy, Pu and δu* decrease with corrosion. These values are extracted from

* P-δ curves and listed in Table 5. It can be noticed that Pu and Py* fit well within experimental

*and numerical results, but P*s does not fit well with the experiment for the uncorroded RC
*beam. Also, for the mid-span deflection, it can be noticed that δy and δu* have a relatively large

*deviation, especially for δy* of the uncorroded beam. The potential cause of this difference is

that the employed constitutive model of concrete underestimates the stiffness of the actual concrete material, which further underestimates the rigidity of the beam.

Concerning the scenario without corrosion, the values for ‘poor bond’ are close to that
of ‘perfect bond’. It demonstrates that it is acceptable to suppose ‘perfect bond’ for the
*uncorroded RC beam; although the values of δy* of both ‘poor bond’ and ‘perfect bond’ do not

fit well with the experiment. However, for the scenario with corrosion, it is noted that the
condition of ‘poor bond’ fits better with the experiment than that of ‘perfect bond’ except for
*P*s, which also indicates the ‘poor bond’ might cause the underestimation of beam stiffness.

**Table 5 Comparisons of mechanical information of experimental data and FEM simulation **

Case
*Ps* *δy* *Py* *δu* *Pu*
Value
(kN) ∆dev
Value
(mm) ∆dev
Value
(kN) ∆dev
Value
(mm) ∆dev
Value
(kN) ∆dev
Exp & no corr 38.7 - 7.6 - 44 - 81.9 - 49.2 -
Poor bond & no corr 32.1 17.2% 11.5 51.3% 46.31 5.3% 97.8 18.4% 49.6 0.8%
Perfect bond & no corr 33.0 14.8% 11.5 51.3% 47 6.8% 102 23.5% 49.6 0.8%
Exp & corr 27.2 - 7.8 - 30 - 35.9 - 37.6 -
Poor bond & corr 26.0 4.5% 8.4 7.7% 30.8 2.7% 40.2 12.0% 39 3.7%
Perfect bond & corr 27.0 0.8% 8.4 7.7% 32 6.7% 43.8 22.0% 39.2 4.3%
Note: ∆dev denotes the |1-computational value/experiment value| × 100%; Exp denotes experimental value

*5.2.2 * *Comparisons of crack patterns *

* Fig. 9 compares the crack patterns of RC beams when achieved the P*u, i.e., ULS, under both
experimental and numerical investigations. For the numerical simulation, cracks are
generated only by loading. Therefore, numerical crack patterns are not reproducing horizontal

**cracks that are mainly due to corrosion (Fig. 9c and d).**

**Comparing uncorroded (Fig. 9a and b) with corroded (Fig. 9c and d) results, it could be **
noticed that the crack patterns, including the crack number, location, and spacing, change
significantly due to the reinforcement corrosion. In the investigated example, the crack width
of the uncorroded scenario is larger than that of the corroded scenario. The primary reason is
*that the crack width of ULS is related to the deformation capacity of the RC beam, e.g., δ*u.
*Both ‘poor bond’ and reinforcement corrosion could impair the δ*u of the RC beam and reduce
the crack width in the investigated case.

due to the difference in strain between the tension bar and concrete in the tensile zone. Under
the assumption of ‘perfect bond’, the strains of tension bars and concrete at the same node are
supposed to be strictly consistent, so their strain and stress distribution are symmetrical on
both sides. However, for ‘poor bond’, without such a strict condition, the strains at the same
node might have some differences. To balance the force matrix and coordinate the element
deformation, the stress and strain distribution on both sides of the beam could be different in
the FEM calculation. Without considering the corrosion effect, this difference has a much
more significant effect on the crack pattern. Besides, for the corroded RC beam, the crack
**pattern is also asymmetric (Figs. 9c and d), and its asymmetry seems much severe than that **
**of the uncorroded RC beam (Figs. 9a and b). Comparing Fig. 9c with d, the bond condition **
does not influence much the crack pattern. Thus, being different from the uncorroded
scenario, the asymmetry of the crack pattern is more due to corrosion non-uniformity than the
bond condition.

(a)

(b)

(c)

(d)

**Fig. 9. Comparisons of crack patterns between experiment and simulation results of different **

scenarios: (a) poor bond & no corr; (b) perfect bond & no corr; (c) poor bond & corr; and (d) perfect bond & corr

lines are simulation results)
*5.2.3 * *Effect of corrosion degree *

In order to investigate the effects of reinforcement corrosion on the simulation results, three corrosion scenarios are supposed:

*(1) original corrosion degree (ηs***) in Fig. 7; **

*(2) 1.1 times the corrosion degree (1.1ηs*) for all steel bar elements; and

*(3) 1.25 times the corrosion degree (1.25ηs*) for all steel bar.

**Table 6 presents the results on the effect of bond condition for the above-mentioned **

*corrosion degrees. It is noted that the bond condition slightly affects Ps, Py, and δy* and does

*not affect δy and P*u of the uncorroded RC beam, as the bond condition of the uncorroded RC
beam is close to ‘perfect bond’. For the corroded RC beam, the effect of bond condition on
*the deflection δ (δu and δy) and load P (Pu and Py*) increases with the corrosion degree, while

*the effect of bond condition on P*s slightly decreases with corrosion degree. Since it is
essential to consider the bond conditions for the mechanical evaluation of corroded RC
beams, the constitutive model of bond-slip (Eqs. (12) and (13)) would be employed for the
sensitivity and reliability analysis.

**Table 6 Comparisons of mechanical information between ‘perfect bond’ and ‘poor bond’ **

Case

*Ps* *δy* *Py* *δu* *Pu*

Value

(kN) ∆dev Value _{(mm) } ∆dev Value _{(kN) } ∆dev Value _{(mm) } ∆dev Value _{(kN) } ∆dev

Perfect bond & no corr 33.0 - 11.5 - 47 - 102 - 49.6 - Poor bond & no corr 32.1 2.8% 11.5 0.0% 46.31 1.5% 97.8 4.1% 49.6 0.0%

Perfect bond & η*s* 27.0 - 8.4 - 32 - 43.8 - 39.2 -

Poor bond & η*s* 26.0 3.7% 8.4 0.0% 30.8 3.8% 40.2 8.2% 39 0.5%

Perfect bond & 1.1η*s* 26.2 - 9.0 - 30.6 - 38.2 - 36.4 -

Poor bond & 1.1η*s* 25.4 3.1% 8.4 6.3% 30 2.0% 27.7 27.5% 35.8 1.6%

Perfect bond & 1.25η*s* 24.9 - 9.6 - 28.4 - 39.5 - 32.2 -

Poor bond & 1.25η*s* 24.2 2.8% 7.9 17.9% 29.2 2.8% 24.3 38.5% 31.8 1.2%

Note: ∆dev denotes the |1- value of ‘Poor bond’/ value of ‘perfect bond’| × 100%

*In order to study the failure mode of a RC beam, the δ values of critical events until *
*reaching δu*, are computed and drawn from the results of FEM simulations, as illustrated in

**breaking, among others., are investigated and plotted in Fig. 10, showing their sequence and **
* corresponding failure modes. In Fig. 10, δu* decreases rapidly with the corrosion degree, and

the chronological order of events varies with the corrosion degrees and bond condition. Given no corrosion, tension bar yields first, then compression bar yields, followed by stirrup yielding, and finally, concrete crushes.

*For the corroded RC beam with the original corrosion degree ηs*, the tension bar breaks

before the concrete crushing, which corresponds with the failure mode reported in [30]. Also,
the event of stirrup bar yielding brings forward; for the 1.25 times of corrosion degree, the
**event of stirrup bar yielding even happens earlier than tension bar yielding. Comparing Fig. **
**10a with Fig. 10b, for the original corrosion degree case η**s, the stirrup bar breaks after δu

under poor bond condition but before the tension bar under perfect bond condition. The
probable cause is the poor bond between the tension bar and concrete, making it easier to
concentrate stress on the tension bar and move its breaking sequence forward. However, after
*1.1ηs*, stirrup bars are severely corroded, leading to the stirrup bar breaking before the tension

bar under both poor and perfect bond conditions. Thus, the failure mode of the RC beam might vary from ductile failure to brittle failure and even from flexural failure to shear failure with corrosion development. Besides, the bond condition might influence the failure mode of the corroded RC beam.

*5.2.4 * *Spatial distribution of cracks and stresses *

The spatial distribution of concrete crack width and the stress of steel bars under ultimate
*load P*u** are investigated in Fig. 11. Fig. 11a presents the distributions of crack width at the **
bottom of the beam. Due to the large deformation development of the uncorroded RC beam,
**its maximum crack width is larger than that of the corroded RC beam. From Fig. 11a, it could **
be noticed that the maximum crack width is not significantly influenced by the corrosion
degree. However, the maximum crack width is affected by the bond condition because poor
bond results in the deformation between concrete and longitudinal bar and simultaneously
increase the crack width of concrete. Therefore, ignoring the bond strength loss might
underestimate the crack width evaluation of the RC beam.

* On the other hand, Fig. 11b shows the stress distribution of longitudinal bars under Pu*,

in which the stresses of the longitudinal bar within the location from 1,170 mm to 1,390 mm
reach the ultimate stress. This result is expected as this zone is mostly affected by the
**corrosion of compressive and tensile bars (Fig. 7). Excepting this critical zone, the stress **
*distribution under load P*u slightly decreases with the corrosion degree.

* In addition, Fig. 11c presents the maximum stress within each stirrup bar under Pu*, in

which only the stirrup bar in the mid-span of the corroded RC beam reaches the ultimate
stress. It is noted that the bond condition influences the stress distribution of stirrup bars. As
*corrosion progresses, more stirrup bars approach ultimate strength. For 1.25ηs*, the perfect

*bond concentrates the stress on the stirrup bars in the mid-span of the beam (m = 6, 7, and 8), *
*but poor bond distributes the stress of stirrup bars discretely (m = 4, 7, and 8). *

**Fig. 11. (a) Crack width distribution at beam bottom; (b) stress distribution of longitudinal **

*bars; and (c) stress distribution of stirrup bars under Pu*

Due to the spatial effects of non-uniform corrosion, the cracking pattern and stress of steel bars are non-uniformly distributed along the RC beam. Corrosion degree mainly influences the deflection and load capacity of the RC beam, the distribution of concrete cracks, and the stress of steel bars. Also, the bond condition affects the distribution of crack and steel bar stress and the deflection and load capacity of corroded RC beam. Thus, realistic modeling of deterioration processes in corroded rebars that considers the spatial variability of corrosion and the bond strength loss of both longitudinal bars and stirrups is paramount for comprehensive condition, lifetime assessment, and failure analysis.

**5.3 PCE-based global sensitivity analysis of RC beams **
*5.3.1 * *Problem description *

Based on the geometry model and loading mode described in Sections 5.1 and 5.2, the
*uncertainties of geometry parameters (L, b, h, and c of the beam, and cross-sectional area of *

*corroded steel bar) and mechanical parameters (f*y*, f*c*, and E*s) on the serviceability and
ultimate capacity are investigated. One deterministic FEM analysis of the RC beam costs
around 10 to 15 minutes by using a PC (CPU: Intel® Core™ i5-8400, 6 Cores; Memory: 16
GB). Thus, MCS, which need a large scale of computations, are costly and not feasible.

In this subsection, a surrogate model based on polynomial chaos expansion (PCE) is
* established. The input variables are given in the following random vector X = [L, b, h, c, fy, fc*,

*E*s**, A**sv**, A**t**, A**c**], where A**sv**, A**t**, and A**c are the vectors of minimum cross-sectional areas of
*stirrup bars [Asv,1, Asv,2, …, Asv,n+1], tension bars [At,1, At,2,…, At,n], and compression bars [Ac,1, *

*Ac,2 ,…, Ac,n*], respectively. Probability distributions of geometry and mechanical parameters

**are listed in Table 7 and those for the cross-sectional area of corroded steel bars are based on **
*the distribution of factor R (Eqs.(6) and (7)). In this study, all random variables are supposed *
to be independent.

**Table 7 Distribution type and values of the parameters **

Parameter Distribution Mean COV Parameter Distribution Mean COV

*L (mm) * Normal 3000 0.01[57] *f*y (MPa) Lognormal 600 0.10[58]

*b (mm) * Normal 150 0.01[57] *f*c (MPa) Normal 42 0.15[59]

*h (mm) * Normal 280 0.01[57] *E*s (MPa) Normal 200000 0.02[60]

*c (mm) * Lognormal 10 0.10[58]
Note: all Normal distributions are truncated at 0.

*The main outputs are the external load P and deflection δ *under different limit states,
including serviceability limit state (SLS) and ultimate limit state (ULS). In general, the SLS
can be expressed through crack width and deflection. In this case, three levels of SLSs are
investigated: SLS1 (crack width = 0.05 mm [61]), SLS2 (*δ = L/500 [62]), and SLS3 (crack *
*width = 1 mm [63]), and three corresponding loads are denoted as P*s1*, P*s2*, and P*s3. For the
*ULS, the ultimate load P*u* of the P-δ curve is collected, and the corresponding failure mode *
can be determined according to the occurrence order of critical events, i.e., the increasing
*sequence of δ under critical events. Based on different corrosion current density i*corr and
*average corrosion degree of steel bars ηave***, 16 scenarios are investigated, as shown in Table 8. **

* Table 8 i*corr

*and ηave*of different cases

No *i*corr _{η}

*ave* No *i*corr *ηave* No *i*corr *ηave* No *i*corr *ηave*

(μA/cm2_{) } _{(μA/cm}2_{) } _{(μA/cm}2_{) } _{(μA/cm}2_{) }

1 0.1 0 5 0.5 0 9 1 0 13 3 0 2 10% 6 10% 10 10% 14 10% 3 30% 7 30% 11 30% 15 30% 4 50% 8 50% 12 50% 16 50%

*5.3.2 * *Comparison between PCE and numerical simulations *

**For each case in Table 8, Monte Carlo simulation (MCS) is performed to create 500 samples; **
*relevant details such as P-δ curves, reinforcement stress, and concrete strain in the *
*compression zone are obtained for further analysis. Taking the i*corr* of 1 μA/cm*2* and ηave* of 10%

* as one example, Fig. 12a compares the simulated P-δ curves with the experimental P-δ curve *
of corroded RC beam. It can be found that the simulation results are close at the elastic stage,

**but their variations increase significantly after the yielding stage. In addition, Fig. 12b shows**

*the histogram of ultimate load P*u from simulated results, and its probability density curve is obtained by the kernel density estimation [64], as well as the mean, maximum and minimum

*value of P at different δ. Also, the experimental P*u, 2.5 %, and 97.5 % quantile values of

*simulated P*u

**and their corresponding PDF values are marked in Fig. 12b. The experimental**

*P*u* is within the 95 % confidence interval of simulated P*u* and close to the simulated peak *
value.

**Fig. 12. (a) PDF contour of simulated P-δ curves and experimental P-δ curves; (b) Histogram **

Furthermore, 400 numerical samples are used to establish the PCE (training set), and the
**other 100 are collected to test the developed PCE (testing set). As shown in Fig. 13, the **
*predicted PCE values of P*s1*, P*s2*, P*s3*, and P*u* are compared with the actual values by using i*corr
*= 0.5 μA/cm*2*_{ as an example. In Fig. 13, the R}*2

_{ of the PCEs for P}s1* and P*s2 range from 0.73 to
*0.99, while the R*2_{ of the PCEs for P}

s3* and P*u* range from 0.84 to 0.96, in which the R*2 of most
scenarios are higher than 0.8.

*On the other hand, regarding the minimum and maximum i*corr* (0.1 and 3 μA/cm*2**), Fig. **

* 14 compares the predictions and actual values of P*s1

*and P*u

**. In Fig. 14, it can be found that**

*i*corr* does not influence P*s1* and P*u* in the case of ηave = 0, but i*corr* affects P*s1* and P*u with the
*degree of corrosion. Besides, the R*2_{ values of P}

s1* and P*u are higher than 0.73 and are not
*widely influenced by i*corr*. The estimated values of R*2 as well as the ability of the PCE
approximations to deal with different corrosion scenarios and limit state functions
demonstrate that this approximation could be used for lifetime assessment and sensitivity
analysis (SA).

* Fig. 13. Comparison between the predictions and actual values under i*corr

*= 0.5 μA/cm*2: (a)

* Fig. 14. Comparison between the predictions and actual values of P*s1

*and P*u:

*(a) P*s1

*, i*corr

*= 0.1 μA/cm*2

*, (b) P*s1

*, i*corr

*=3 μA/cm*2,

*(c) P*u*, i*corr*= 0.1 μA/cm*2*, and (d) P*u*, i*corr* = 3 μA/cm*2

The random distribution of the target physical variables could be easily obtained through
a MCS with 106_{ simulations from the PCE model. For instance, Fig. 15 depicts the PDF of }*the original simulations and PCE for i*corr* = 3 μA/cm*2**. As seen in Fig. 15, the PDFs of PCE **
obtained by the training set fit well with the discrete PDF of 500 simulations. These results
are useful for computing the reliability under different limit states of a corroded beam
subjected to a given external load and different corrosion degrees.

* Fig. 15. Comparison between PDF of actual and PCE values for i*corr

*= 3 μA/cm*2

*: (a) P*s1, (b)

*P*s2*, (c) P*s3*, and (d) P*u

*5.3.3 * *Failure probability with respect to different failure modes *

The comprehensive numerical model allows establishing the occurrence of critical events for
**different corrosion levels, as illustrated in Fig. 10. PCE enables the development of surrogate **
models for the external loads associated with the three failure modes, i.e., stirrup breaking,
longitudinal bar breaking, and concrete crushing. Given the input information, the values of
three loads can be evaluated and compared to determine the failure mode by the method
described in Section 5.2.3. In addition, by combining with MCS, these surrogate models can
*be used to evaluate the probability of occurrence of these three failure modes Pf1* (stirrup

*breaking), Pf2 (tension bar breaking), and Pf3* (concrete crushing).

**Based on the failure events for each mode, Fig. 16 illustrates the contribution of each **
failure mode for different corrosion scenarios. It is found that the failure mode of an
uncorroded RC beam is dominated by concrete crushing. Besides, the failure mode of a
corroded RC beam varies with the corrosion degree and corrosion rate, which could be
summarized as follows:

(1) For *η*ave* = 10%, the failure mode is dominated by tension bar breaking (Pf2* = 53% to

*72%). Besides, Pf2 decreases with i*corr*, while Pf1 increases with i*corr*, and Pf3* remains basically

(2) For *η*ave* = 30 %, the failure mode is still dominated by tension bar breaking (Pf2* = 86%

to 89 %) is much higher than the scenario of *η*s* = 10%. The values of Pf1, Pf2, and Pf3* are

*literally unchanged with i*corr; and

(3) For *η*ave* = 50 %, Pf2 is still the largest (Pf2 = 66% to 82%), but Pf1* becomes higher

than the scenario of *η*ave* = 30%. Meanwhile, Pf2 increases with i*corr*, while Pf1* decreases with

*i*corr*, and Pf3* changes a few.

*i*corr* η*ave
*(μA/cm*2_{) } 0 0.1 0.3 0.5
0.1
0.5
1
3